Research Article | Open Access
Pham Van Viet, Cao Minh Thi, Le Van Hieu, "The High Photocatalytic Activity of SnO2 Nanoparticles Synthesized by Hydrothermal Method", Journal of Nanomaterials, vol. 2016, Article ID 4231046, 8 pages, 2016. https://doi.org/10.1155/2016/4231046
The High Photocatalytic Activity of SnO2 Nanoparticles Synthesized by Hydrothermal Method
Tin oxide nanoparticles (SnO2 NPs) were prepared at low temperature by hydrothermal method. Synthesized SnO2 NPs were confirmed via characterization techniques such as UV-visible spectroscopy (UV-vis), X-ray diffraction (XRD), and Transmission Electron Microscope (TEM). The synthesized nanoparticles were in the size of 3 nm and they have high photocatalytic activity. The result showed that SnO2 NPs degraded 88.88% MB solution after 30 minutes of UV illumination and reached 90.0% for 120 minutes (2 hours) of UV illumination. Moreover, they degraded 79.26% MB solution after 90 minutes (1.5 hours) under assisted sunlight illumination.
In recent years, nanomaterials attracted much attention due to their high surface-to-volume ratio, enhanced characteristics of quantum size effects, and the high fraction of chemically similar surface sites . Among metal oxide semiconductor materials, tin dioxide (SnO2) has been attracting a great deal of research interest owing to its outstanding physical and chemical properties [2–4]. SnO2 is an n-type semiconductor with a wide band gap of 3.6 eV at room temperature, having excellent optical and electrical properties such as peculiar optical transparency, low resistivity, and high theoretical specific capacity [5, 6]. Moreover, SnO2 possesses a high electron mobility (~100–200 cm2 V−1s−1), indicating a faster transport of photoexcited electrons [7–9]. In the last decade, SnO2 has been studied as promising material with many unique surface properties including luminescence and photocatalytic activity . In particular, as the diameter of SnO2 is smaller than excitons and carriers are confined in all three dimensions to a nanometer size region, the high band gap energy and high stability of SnO2 nanoparticles (SnO2 NPs), unique properties such as the blue shift of the band edge transition energy, and unusual structural and optical properties take place [10, 11]. Moreover, the high degradation rate of the organic dye on the as-synthesized SnO2 NPs with size below 10 nm can be attributed to the small size of SnO2 NPs because the large surface area helps to increase the photocatalytic reaction sites and promotes the efficiency of the electron-hole separation [12–14].
There are many methods to synthesize SnO2 NPs, such as sol-gel [2, 15], hydrolysis , electrochemical oxidation of tin metal sheet in a nonaqueous electrolyte containing NH4F , the chemical coprecipitation route [18, 19], dropping ammonium hydroxide into tin salt solution under sonication , and a microwave irradiation method [21, 22]. However, the hydrothermal method with an aqueous solvent as a reaction medium is environmentally friendly because the reactions are carried out in a closed system. Hydrothermal synthesis involves use of water as a solvent at elevated temperatures and pressures in a closed system and certain properties of the solvents such as density, viscosity, and diffusion coefficient change [23, 24]. Furthermore, hydrothermal synthesis is often used due to its simple processes and equipment, without high temperature sintering, allowing the control of the grain size, morphology, and degree of crystallinity by easy changes in the experimental procedure .
In the present work, we synthesize SnO2 NPs powder via a simple hydrothermal method from tin chloride, sodium hydroxide, and hydrazine hydrate. The trick in the hydrothermal method presented here is the application of hydrazine hydrate (N2H4·H2O), which served as both the alkali and the ligand to coordinate with Sn ions to form a complex cluster. Furthermore, the hydrothermal process is desirable for the large-scale fabrication of other ultrafine oxide nanoparticles . Besides, the photodegradation of dye organics by solar irradiation is a comparatively greener approach than by UV-light . Previous publications on the photocatalytic activity of SnO2 NPs often use UV-light as excited source for photoreactions. Herein, we synthesized SnO2 particles with diameters <10 nm, which presents excellent photocatalytic degradation using MB as a model pollutant in the presence of UV-light and direct sunlight.
Tin chloride (SnCl4·5H2O, Merck, 99.99% pure), hydrazine hydrate (N2H4·H2O, 99% pure), sodium hydroxide (NaOH, 99%), methanol (CH3OH, 99% pure), and methylene blue (C16H18N3SCl, JHD Fine Chemicals, China, 99%) were used. Deionized (DI) water was obtained from Thermal Scientific.
2.2. Synthesis of SnO2 NPs by the Hydrothermal Method
SnO2 NPs were prepared using the hydrothermal method. Firstly, 0.9028 g SnCl4·5H2O was introduced into a mixed solution of 25.75 mL DI water and 1.14 mL hydrazine hydrate (N2H4·H2O). After that, solutions were adjusted to pH = 12 by the addition of the NaOH solution and transferred to a stainless autoclave. Finally, it is heated at 135°C for 24 hours and cooled naturally to room temperature. The product was centrifuged, filtered out, rinsed with methanol and DI water several times, and then dried at 120°C for an hour in the air.
2.3. Characterization of SnO2 NPs
The size and morphology of SnO2 NPs were characterized by TEM (JEM 1400 Instrument, JEOL). XRD analysis was carried out (Bruker D8-Advance 5005) at a voltage of 45 kV with Cu Kα radiation (λ = 1.5406 Å) to examine the crystalline phase of synthesized nanoparticles. The Fourier transform infrared spectroscopy (FT-IR) spectrum was recorded on a FT-IR spectrometer (Vertex 80, Bruker, Germany) over the range of 400 to 4 000 cm−1 in transmission mode at room temperature to identify the functional group present on SnO2 NPs and responsible for the stability of nanoparticles.
2.4. Photocatalytic Activity of SnO2 NPs for Degradation of the MB Solution
In order to determine the photocatalytic activity of the SnO2 NPs, we use the MB dye solution as a model of contamination to characterize their photocatalytic activity. In the experiment, 30 mL of the MB solution (10 mg/L) and 0.03 grams of catalyst were used. This solution was stirred for 10 minutes in dark for the equilibrium of the adsorption and desorption process of MB with NPs. After stirring, the solution was irradiated by UV lamp (Osram, Germany) and direct sunlight conditions. The UV lamp has radiation of 350 nm with 7 W of lamp power. Concentrations of the MB solution initially and after every 15 minutes of irradiation of UV-light were taken by using UV-visible spectrophotometer (U2910, Hitachi, Japan). In case these solutions irradiated by sunlight, the experiments were carried out on a sunny day at Ho Chi Minh City between 10 a.m.–1 p.m. with outside temperature from 35°C to 40°C and these experiments were tested 3 times.
3. Results and Discussion
3.1. X-Ray Diffraction (XRD) Pattern Analysis
The XRD pattern of the product is shown in Figure 1. The peaks at 2θ values of 26.6°, 33.8°, 51.8°, and 65.9° can be associated with (110), (101), (211), and (301), respectively. A matching of the observed and standard planes confirmed that the product is of SnO2 having a tetragonal structure, which are in good agreement with the literature values (JCPDS card number 41-1445). The average particle size () was estimated using the following Scherrer equation [30, 31]:where is the crystallite size, λ is the X-ray wavelength, β is the full width at half maximum of the diffraction peak, and θ is the Bragg diffraction angle of the diffraction peaks. The average particle size of SnO2 calculated using Scherrer equation of SnO2 is 3 ± 0.1 nm.
Comparison of the XRD pattern of the as-synthesized samples is as follows: the samples calcined at 300°C in flowing air for 2 hours (Figure 1(b)) do not change characterization peaks of SnO2 peaks and the intensity of peaks do not increase significantly. Therefore, we only use the as-synthesized samples for survey continuously.
3.2. Transmittance Electron Microscopic Analysis (TEM)
The morphology and the particles size of the samples were obtained by TEM images (Figure 2(a)). The image shows that spherical shaped nanoparticles have been formed and they were uniformly distributed except for a few aggregated particles. The diameter of SnO2 Nps measured from TEM image is in the range of 0.5–5.5 nm with an average of 2.2 nm which is almost the same as that obtained from XRD patterns (Figure 2(b)).
3.3. Fourier Transform Infrared Spectroscopy
The FT-IR spectroscopy was recorded at room temperature for determination of the functional group of materials available in the nanopowders. The FT-IR spectrometer was used for the analysis in a range between 4000 and 380 cm−1, as shown in Figure 3. The band around 3454.29 to 3539.64 cm−1 and 1612.43 cm−1 indicates the presence of O-H group due to stretching vibrations of water molecules or hydroxyl groups absorbed at the surface of SnO2 and also to stretching vibrations of Sn-OH groups [26, 32]. The band around 3196.74 cm−1 and 2928.99 cm−1 indicates the presence of C-H group. The peak around 608.14 cm−1 is assigned to Sn-O-Sn stretching mode of surface bridging oxide formed by the condensation of adjacent surface hydroxyl groups [25, 26, 32]. Therefore, the presence of these bands confirmed the formation of SnO2.
3.4. Photocatalytic Activity of SnO2 NPs
The photocatalytic activity of SnO2 NPs was examined by the changes in the absorption spectra of the MB dye solution during their photodegradation process. Figure 4(a) shows that commercial SnO2 degraded of 20.49% MB solutions after 30 minutes of UV lamp illumination and it mostly does not degrade when increasing illumination time. Figures 4(b) and 4(c) show the change of the absorption of MB solution when it obtained SnO2 NPs under different UVA irradiation times. Figure 4(b) shows that the degradation activity of SnO2 NPs is better than the commercial SnO2. Figure 4(c) is a magnified image of Figure 4(b). It shows that the typical absorption peak of MB at 664 nm wavelength is significantly decreased. However, when the irradiation time increases from 15 minutes to 180 minutes, the decline of the absorption peak of MB is insignificant. Besides, Figures 4(b) and 4(c) indicate that SnO2 NPs degraded 88.88% MB solution after 30 minutes of UV illumination and reached 90.0% for 120 minutes (2 hours) of UV illumination. These results shows that the more the illumination time increases, the more the concentration of MB dye decreases, which is shown by the decrease in UV-absorbance spectra. It can be seen that the intensity of the absorption peak gradually decreases with increasing UV illumination time.
Figure 5 shows the photocatalytic activity of SnO2 NPs according to UV illuminated times condition. After 15 minutes of UV illumination, SnO2 NPs degraded strongly MB solutions and nearly saturated during the time from 30 minutes to 180 minutes. Whereas, the degradation of commercial SnO2 is weak and unstable.
Because SnO2 Nps are synthesized by hydrothermal method, there are the generated oxygen vacancies in SnO2 crystal, and these can induce the formation of new energy levels in the band gap. After the heat treatment of Sn(OH)4, the hydroxyls remaining in the structure will generate molecular water, while releasing the lattice oxygen and producing a neutral oxygen vacancy () in its position. Also the high pressure produced in the hydrothermal process is in favor of the removal of hydroxyls and production oxygen vacancies. The process can be expressed as follows:orThese neutral vacancies may be singly ionized vacancies as or . Semiconductor photocatalytic activity has attracted great interest due to its potential applications in the degradation of environmental pollutants and organic pollutant transformation.
So, electron (e−) is excited from the valence band into the conduction band, generating hole (h+) when a photon with energy of matches or exceeds bandgap energy, , of semiconductor SnO2:In the photocatalytic reaction, and radicals are the extremely strong reduction and oxidation agent, respectively.
Figure 6 shows the UV-visible absorbance spectra for the photodegradation of MB dye of commercial SnO2 and SnO2 NPs under direct sunlight. Sunlight assisted photodegradation property of SnO2 NPs was investigated and it shows the photodegradation efficiency of 79.26% MB solution after 90 minutes (1.5 hours) under direct sunlight illumination. Otherwise, the commercial SnO2 powder only degrades 36.23% of MB solution. Besides, we compared with previous studies of other researchers for the photocatalytic degradation of MB using SnO2 NPs. These results show that the degradation ability of SnO2 NPs with MB solution is very high under both UV illumination and sunlight. It is indicated that only a very small amount of SnO2 NPs (0.03 grams) was degradable more over 90% MB solution under UV illumination condition (power of lamp is 7 W) for 2 hours.
A comparison between the present study and studies conducted by other researchers is shown in Table 1. The comparison also showed that the synthesized SnO2 NPs in this research have extremely high photocatalytic activity.
SnO2 NPs of average size 3 nm synthesized by hydrothermal method from tin chloride, sodium hydroxide, and hydrazine hydrate. The photodegradation efficiency of SnO2 NPs with MB solution is very high under both UV illumination and sunlight. SnO2 NPs degraded strongly MB solutions (>80.0%) after 15 minutes of UV illumination and degraded 79.26% MB solution after 90 minutes under sunlight irradiation.
The authors declare that they have no competing interests.
The authors thank members of The CM Thi Lab for assistance with the UV-vis absorption spectra. This research is funded by Vietnam National University, Ho Chi Minh City (VNU-HCM), under Grant no. C2014-18-14.
- H. Zhu, D. Yang, G. Yu, H. Zhang, and K. Yao, “A simple hydrothermal route for synthesizing SnO2 quantum dots,” Nanotechnology, vol. 17, no. 9, pp. 2386–2389, 2006.
- E. Abdelkader, L. Nadjia, and V. Rose-Noëlle, “Adsorption of Congo red azo dye on nanosized SnO2 derived from sol-gel method,” International Journal of Industrial Chemistry, vol. 7, no. 1, pp. 53–70, 2016.
- N. Srivastava and M. Mukhopadhyay, “Biosynthesis of SnO2 nanoparticles using bacterium Erwinia herbicola and their photocatalytic activity for degradation of dyes,” Industrial & Engineering Chemistry Research, vol. 53, no. 36, pp. 13971–13979, 2014.
- A. Nazari and S. Riahi, “The effects of SnO2 nanoparticles on physical and mechanical properties of high-strength self-compacting concrete,” Journal of Experimental Nanoscience, vol. 7, no. 5, pp. 559–577, 2012.
- S. Sheng Pan, S. Fung Yu, Y. Xia Zhang et al., “Crystallite size-modulated exciton emission in SnO2 nanocrystalline films grown by sputtering,” Journal of Applied Physics, vol. 113, no. 14, Article ID 143104, 2013.
- L. Shi and H. Lin, “Facile fabrication and optical property of hollow SnO2 spheres and their application in water treatment,” Langmuir, vol. 26, no. 24, pp. 18718–18722, 2010.
- X. Xu, G. Yang, J. Liang et al., “Fabrication of one-dimensional heterostructured TiO2@SnO2 with enhanced photocatalytic activity,” Journal of Materials Chemistry A, vol. 2, no. 1, pp. 116–122, 2014.
- F. Cai, Z. Yuan, Y. Duan, and L. Bie, “TiO2 coated SnO2 nanosheet films for dye-sensitized solar cells,” Thin Solid Films, vol. 519, no. 16, pp. 5645–5648, 2011.
- C. Gao, X. Li, B. Lu et al., “A facile method to prepare SnO2 nanotubes for use in efficient SnO2-TiO2 core-shell dye-sensitized solar cells,” Nanoscale, vol. 4, no. 11, pp. 3475–3481, 2012.
- E. J. H. Lee, C. Ribeiro, T. R. Giraldi, E. Longo, E. R. Leite, and J. A. Varela, “Photoluminescence in quantum-confined SnO2 nanocrystals: evidence of free exciton decay,” Applied Physics Letters, vol. 84, no. 10, pp. 1745–1747, 2004.
- H.-J. Ahn, H.-C. Choi, K.-W. Park, S.-B. Kim, and Y.-E. Sung, “Investigation of the structural and electrochemical properties of size-controlled SnO2 nanoparticles,” The Journal of Physical Chemistry B, vol. 108, no. 28, pp. 9815–9820, 2004.
- S. Wu, H. Cao, S. Yin, X. Liu, and X. Zhang, “Amino acid-assisted hydrothermal synthesis and photocatalysis of SnO2 nanocrystals,” The Journal of Physical Chemistry C, vol. 113, no. 41, pp. 17893–17898, 2009.
- X. Xu, J. Zhuang, and X. Wang, “SnO2 quantum dots and quantum wires: controllable synthesis, self-assembled 2D architectures, and gas-sensing properties,” Journal of the American Chemical Society, vol. 130, no. 37, pp. 12527–12535, 2008.
- V. T. Agekyan, “Spectroscopic properties of semiconductor crystals with direct forbidden energy gap,” Physica Status Solidi (A) Applied Research, vol. 43, no. 1, pp. 11–42, 1977.
- M. Dimitrov, T. Tsoncheva, S. Shao, and R. Köhn, “Novel preparation of nanosized mesoporous SnO2 powders: physicochemical and catalytic properties,” Applied Catalysis B: Environmental, vol. 94, no. 1-2, pp. 158–165, 2010.
- S. de Monredon, A. Cellot, F. O. Ribot et al., “Synthesis and characterization of crystalline tin oxide nanoparticles,” Journal of Materials Chemistry, vol. 12, no. 8, pp. 2396–2400, 2002.
- W. Chen, D. Ghosh, and S. Chen, “Large-scale electrochemical synthesis of SnO2 nanoparticles,” Journal of Materials Science, vol. 43, no. 15, pp. 5291–5299, 2008.
- P. P. Sahay, R. K. Mishra, S. N. Pandey, S. Jha, and M. Shamsuddin, “AC transport properties of nanocrystalline SnO2 semiconductor,” Ceramics International, vol. 38, no. 2, pp. 1281–1286, 2012.
- V. Senthilkumar, P. Vickraman, M. Jayachandran, and C. Sanjeeviraja, “Synthesis and characterization of SnO2 nanopowder prepared by precipitation method,” Journal of Dispersion Science and Technology, vol. 31, no. 9, pp. 1178–1181, 2010.
- G. Pang, S. Chen, Y. Koltypin, A. Zaban, S. Feng, and A. Gedanken, “Controlling the particle size of calcined SnO2 nanocrystals,” Nano Letters, vol. 1, no. 12, pp. 723–726, 2001.
- M. Parthibavarman, V. Hariharan, and C. Sekar, “High-sensitivity humidity sensor based on SnO2 nanoparticles synthesized by microwave irradiation method,” Materials Science and Engineering C, vol. 31, no. 5, pp. 840–844, 2011.
- S. Sain, A. Kar, A. Patra, and S. K. Pradhan, “Structural interpretation of SnO2 nanocrystals of different morphologies synthesized by microwave irradiation and hydrothermal methods,” CrystEngComm, vol. 16, no. 6, pp. 1079–1090, 2014.
- K. Jain, A. Shrivastava, and R. Rashmi, “Synthesis and controlling the morphology of SnO2 nanocrystals via hydrothermal treatment,” ECS Transactions, vol. 1, pp. 1–7, 2006.
- Y. Wang, L. Tan, and L. Wang, “Hydrothermal synthesis of SnO2 nanostructures with different morphologies and their optical properties,” Journal of Nanomaterials, vol. 2011, Article ID 529874, 10 pages, 2011.
- X. Cao, Y.-C. Shu, Y.-N. Hu, G.-P. Li, and C. Liu, “Integrated process of large-scale and size-controlled SnO2 nanoparticles by hydrothermal method,” Transactions of Nonferrous Metals Society of China, vol. 23, no. 3, pp. 725–730, 2013.
- A. Bhattacharjee, M. Ahmaruzzaman, and T. Sinha, “Surfactant effects on the synthesis of durable tin-oxide nanoparticles and its exploitation as a recyclable catalyst for the elimination of toxic dye: a green and efficient approach for wastewater treatment,” RSC Advances, vol. 4, no. 93, pp. 51418–51429, 2014.
- G. Elango, S. M. Kumaran, S. S. Kumar, S. Muthuraja, and S. M. Roopan, “Green synthesis of SnO2 nanoparticles and its photocatalytic activity of phenolsulfonphthalein dye,” Spectrochimica Acta Part A: Molecular and Biomolecular Spectroscopy, vol. 145, pp. 176–180, 2015.
- N. Talebian and F. Jafarinezhad, “Morphology-controlled synthesis of SnO2 nanostructures using hydrothermal method and their photocatalytic applications,” Ceramics International, vol. 39, no. 7, pp. 8311–8317, 2013.
- A. Bhattacharjee and M. Ahmaruzzaman, “Photocatalytic-degradation and reduction of organic compounds using SnO2 quantum dots (via a green route) under direct sunlight,” RSC Advances, vol. 5, no. 81, pp. 66122–66133, 2015.
- B. D. C. S. R. Stock, Elements of X-Ray Diffraction, Prentice-Hall, 3rd edition, 2001.
- G. E. Patil, D. D. Kajale, V. B. Gaikwad, and G. H. Jain, “Preparation and characterization of SnO2 nanoparticles by hydrothermal route,” International Nano Letters, vol. 2, no. 1, p. 17, 2012.
- S. Lenaerts, J. Roggen, and G. Maes, “FT-IR characterization of tin dioxide gas sensor materials under working conditions,” Spectrochimica Acta Part A: Molecular and Biomolecular Spectroscopy, vol. 51, no. 5, pp. 883–894, 1995.
- S. K. Kansal, M. Singh, and D. Sud, “Studies on photodegradation of two commercial dyes in aqueous phase using different photocatalysts,” Journal of Hazardous Materials, vol. 141, no. 3, pp. 581–590, 2007.
- H. Cao, X. Qiu, Y. Liang, L. Zhang, M. Zhao, and Q. Zhu, “Sol-gel template synthesis and photoluminescence of n- and p-type semiconductor oxide nanowires,” ChemPhysChem, vol. 7, no. 2, pp. 497–501, 2006.
Copyright © 2016 Pham Van Viet et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.